Desalination xxx (xxxx) xxx–xxx
Contents lists available at ScienceDirect
Desalination journal homepage: www.elsevier.com/locate/desal
Removal of strontium from aqueous solutions and synthetic seawater using resorcinol formaldehyde polycondensate resin T. Nur, P. Loganathan, J. Kandasamy, S. Vigneswaran⁎ Faculty of Engineering, University of Technology Sydney (UTS), P.O. Box 123, Broadway, NSW 2007, Australia
A R T I C L E I N F O
A B S T R A C T
Keywords: Adsorption Radioactive waste Resorcinol formaldehyde Seawater Strontium Zeta potential
Strontium (Sr) is a valuable metal found in abundance in seawater. However, its recovery from seawater has received little attention despite its many industrial applications. Batch and column adsorption experiments were conducted on the removal of Sr by resorcinol formaldehyde (RF) resin in the presence of co-existing cations at pH 7.5–8.5, where maximum adsorption was found. Batch adsorption capacities of cations followed the decreasing order of Sr > Ca > Mg > K, the order being the same as that of reduction of negative zeta potential. The adsorption data for Sr, Ca and Mg satisfactorily ﬁtted to the Langmuir adsorption model with maximum adsorption capacities of 2.28, 1.25 and 1.15 meq/g, respectively. Selectivity coeﬃcients for Sr with respect to other metals showed that Sr was selectively adsorbed on RF. Column adsorption data for Sr only solution ﬁtted well to the Thomas model. Sr adsorption capacity in the presence of seawater concentrations of Ca, Mg, K and Na was reduced in both batch and column experiments with highest eﬀect from Ca and Mg. However, if Ca and Mg are removed prior to RF adsorption process by precipitation, the negative eﬀect of these ions on Sr removal can be signiﬁcantly reduced.
1. Introduction Seawater is becoming an important source of several valuable mineral resources because of the depletion of high-grade mineral ores on land and recent problems associated with land-based industries resulting from sustainable water and energy demand and environmental issues . Due to its large reserve, seawater is an attractive resource for valuable minerals such as lithium, uranium, rubidium, and strontium (Sr) despite their very low concentrations. Among these valuable minerals, Sr is one of the most abundant minerals in seawater with an average concentration of 6–7 mg/L . Strontium, which is an alkaline earth metal, has many industrial applications, such as in ceramic ferrite magnets, ceramics, glass and pyrotechnics industries, ﬂuorescent lights and ﬁre-works, and also for drilling mud in the oil and gas industries [1,3]. To date, however, the recovery of Sr from seawater has received little attention despite its many industrial applications. Moreover, the removal of Sr from radioactive waste water is a very critical issue as it is considered one of the most dangerous radionuclides to human health due to its high solubility, transferability, and easy assimilation [4,5]. Strontium has four major naturally occurring stable isotopes: 84Sr, 86Sr, 87Sr and 88Sr in addition to 31 unstable isotopes and the longest-lived unstable isotope is 90Sr with a half-life of 28.9 years. The 90Sr isotope is a beta-emitter that genetically aﬀects seawater
organisms and ultimately causes harm to humans . Removing radioactive Sr from seawater is also important particularly since the Fukushima nuclear plant accident in 2011, which led to serious seawater contamination by radioactive strontium 90Sr [7,8]. Strontium genetically impacts on seawater organisms and eventually causes serious damage to humans. In countries like the USA, Jordan and Japan, Sr contamination in groundwater and other water sources has been reported and the United States Environmental Protection Agency (U.S. EPA) has recommended a permissible limit of 4.0 mg/L of Sr in drinking water . High Sr concentrations in drinking water sources may potentially lead to many diseases increasing, including neurological disorders ranging from learning disabilities to severe mental retardation . It is therefore important to develop appropriate removal techniques for the removal of Sr from water both to decontaminate waters and to recover Sr for beneﬁcial uses. Of the various methods for removing Sr such as solvent extraction , adsorption [12,13], ion exchange , electrocoagulation , and membrane ﬁltration , adsorption/ion exchange is a promising method for removing Sr from seawater and radioactive wastewaters because of its potential to separate Sr from seawater despite the low concentration levels of this metal, low cost, and a simple process to implement with less chemical waste production. As ion exchange is one type of adsorption process which leads to adsorption of ions , in
Corresponding author. E-mail address: [email protected]
http://dx.doi.org/10.1016/j.desal.2017.08.003 Received 2 March 2017; Received in revised form 2 August 2017; Accepted 2 August 2017 0011-9164/ © 2017 Elsevier B.V. All rights reserved.
Please cite this article as: Nur, T., Desalination (2017), http://dx.doi.org/10.1016/j.desal.2017.08.003
Desalination xxx (xxxx) xxx–xxx
T. Nur et al.
R − OH + AOH → R–O − A + H2 O
this paper it is discussed under the general process of adsorption. Different studies have been conducted to investigate Sr adsorption using various adsorbents such as hydrous ferric oxide , dolomite , strontium-ion imprinted hybrid gel , alginate-based biosorbent  and titanosilicate . Not all adsorbents, however, were found to have high adsorption capacities. Moreover, most of these Sr adsorption studies were conducted in batch experiments and not in column experiments which are more appropriate for practical application. Resorcinol formaldehyde (RF) resin is an eﬀective phenolic resin which is formed by the polycondensation of resorcinol and formaldehyde in alkaline solution . Commercial phenol formaldehyde resins – similar to RF resin – were utilised to treat low and high level alkaline radioactive wastes , as well as laboratory synthesised phenol formaldehyde resins for the removal of both Cs and Sr from radioactive wastewaters . Previous research reported that the phenol formaldehyde resins that are similar to RF resin were generally conditioned with alkaline solutions. This is because the main functional weakly acidic phenolic –OH groups of the resin responsible for ion exchange were expected to fully realise their ion-exchange properties only if the –OH groups were ionised to the highest extent which occurs in alkaline solutions . It was reported that RF resin could be used to simultaneously adsorb Sr along with Cs from radioactive waste solutions , but Banerjee et al.  found that the RF resin used in their study was highly selective for the removal of Cs compared to Sr from simulated radioactive waste solution. However, no detailed study has been done on Sr removal and recovery from seawater using RF resin, especially in the presence of co-ions using both batch and column methods. The concentration of Cs (4–50 × 10− 5 M) is much higher than that of Sr (3–15 × 10− 7 M) in radioactive wastewater . Therefore, Cs was preferentially adsorbed on RF. However, in seawater, the opposite is expected to occur because Sr concentration (1 × 10− 4 M) is much higher than that of Cs (6 × 10− 9 M) . The objectives of this study were to: (i) synthesise and evaluate the performance of RF resin for Sr adsorption in batch and column adsorption methods; (ii) evaluate the pH eﬀect on Sr adsorption and study the adsorption mechanism using zeta potential measurements; (iii) investigate the eﬀect of co-ions in seawater on Sr adsorption using synthetic seawater in batch and column adsorption methods; and (iv) evaluate the Sr desorption characteristics of the RF resin to obtain useful information on Sr recovery.
2 R − OH + B (OH)2 → (R − O)2 − B + 2H2 O
where R is the resorcinol formaldehyde polymer and A is Na or K+ and B is Ca++. Based on earlier research on the adsorption of Cs by RF resin, it can be said that the phenolic OH group of the resin is ionised to phenolate ion under alkaline conditions [23,26,30] and then it participates in ion exchange reaction of Sr. The uptake of Sr ions by the resin conditioned with Na+, K+, Ca++ is shown by similar ion exchange reactions in Eqs. (3), (4).
2 R–O − A + Sr++ → (R − O)2 − Sr + 2A+
(R − O)2 − B + Sr++ → (R − O)2 − Sr + B++
The virgin and the three RF resins conditioned with NaOH, KOH and Ca(OH)2 were used in the adsorption experiments. 2.2. RF resin characterisation Zeta potential is an important parameter for understanding the mechanism of adsorption as it is the electrical potential close to a particle surface where adsorption of ions from solution phase occurs and it is positively related to the surface charge. The zeta potential values were measured on 0.5 g/L of RF resin suspensions in the presence of 10− 3 M of NaCl, KCl, CaCl2, MgCl2, or SrCl2 in the pH range of 2.5–10.0 using a Zetasizer nano instrument (Nano ZS Zen3600, Malvern, UK). Triplicate measurements were made to minimise undesirable biases (with diﬀerences between replicates always being < 5%) and the average value was used for data analyses. RF resin was also characterised using X-ray diﬀraction (XRD) and Fourier transform infrared (FTIR) spectroscopy. The FTIR pattern was obtained using a Miracle-10 Shimadzu FTIR spectrometer. The spectra were obtained at 4 cm− 1 resolution by measuring the absorbance from 400 to 4000 cm− 1 using a combined 40 scans. XRD was carried out using a PANalytical Empyrean instrument operated at 60-kV with CuKa1 radiation on powdered samples of RF resin. Ion exchange capacity of the RF resin was measured using two methods [23,28]. In both methods, the RF was equilibrated with known concentrations of NaOH and NaCl and the amounts of NaOH consumed in the ion exchange reaction were determined by titrating the remaining NaOH with 0.1 M HCl using phenolphthalein indicator. The measurements were made in triplicate and the average values were recorded.
2. Materials and method 2.1. Adsorbents
2.3. Feed solutions and chemical analysis
The main adsorbent used in this study was RF resin but four other commercially available adsorbents namely CsTreat, ammonium molybdophosphate (AMP), Zeolite, and Amberlite FPC 3500 were also used to compare their Sr adsorption capacities [28,29]. RF resin was prepared by following the procedure described by Samanta et al.  where a mixture of solutions with resorcinol: formaldehyde: NaOH: H2O mole ratio of 1:2.5:1.5:50 was used. The dark-red coloured mixed solution was then oven dried at 100 °C for 24 h and the dried reddish brown RF resin was ground and sieved to 0.25–0.45 mm particle size. The sieved RF resin was then washed with 1 M HCl to convert RF resin to an acid form (H+). After that, the resin was washed thoroughly with MQ water to convert it to a neutral form and dried at room temperature (24 ± 1 °C) for 24 h. To increase the ion exchange capacity, the H+ form of the resin was conditioned separately with alkaline solutions of 1 M NaOH, KOH and Ca(OH)2 by shaking 5 g of the resin in 500 mL solution of each of the metal hydroxides separately at 150 rpm for 24 h. Following that, the resin was thoroughly washed with MQ water to remove excess NaOH, KOH and Ca(OH)2 and then dried at room temperature (24 ± 1 °C) for 24 h and kept stored in air tight containers. The reactions involved in the conditioning of RF resin with the diﬀerent metal hydroxides are given in Eqs. (1), (2).
Feed solutions were prepared using analar grade chemicals - KCl, NaCl, CaCl2, MgCl2 and SrCl2 (Sigma-Aldrich) - at pH 7.5–8.5. Sr, K, Na, Ca, and Mg concentrations were determined using Microwave Plasma Atomic Emission Spectroscopy (MP-AES) (Agilent 4100). 2.4. Batch adsorption experiments 2.4.1. Sr adsorption by diﬀerent RF resins The ﬁrst batch experiment was conducted with virgin RF resin and RF resin conditioned separately with NaOH, KOH, and Ca(OH)2 at adsorbent doses of 0.1–1.0 g/L and ﬁxed Sr concentration of 10 mg/L to select the adsorbent having the highest Sr adsorption capacity. The amount of Sr adsorbed at equilibrium, qe (mg/g), was calculated using Eq. (5).
(C0 − Ce )V M
where C0 = initial concentration of Sr (mg/L); Ce = equilibrium concentration of Sr (mg/L); V = volume of the solution (L); and M = mass 2
Desalination xxx (xxxx) xxx–xxx
T. Nur et al.
concentration of the metal in solution (meq/L) [23,25,28] and the selectivity coeﬃcient of Sr with respect to another metal (Ks) was determined by dividing the Kd of Sr by the Kd of the other metal . The higher the Ks value of Sr, the higher the selectivity of adsorption of Sr with respect to the other metal.
of adsorbent (g). As RF resin conditioned with NaOH had the highest Sr adsorption capacity among the four resins (Fig. S1), the subsequent adsorption experiments were conducted with this resin only. 2.4.2. Sr adsorption by diﬀerent commercial adsorbents Equilibrium adsorption experiments were conducted in a set of glass ﬂasks with 100 mL solutions of pH 7.5–8.5 containing Sr at a concentration of 10 mg/L that is approximately the same as the Sr concentration in seawater. Four commercially available adsorbents (CsTreat, AMP, Zeolite and Amberlite FPC 3500) at doses of 0.1–10 g/L were added to the solutions and agitated as before in a ﬂat shaker to determine their relative Sr adsorption capacities. At the end of the shaking period of 24 h, the samples were ﬁltered and the ﬁltrates were analysed for Sr concentration. The amount of Sr adsorption was calculated using Eq. (5).
2.5. Column adsorption experiments The column adsorption experiments were done using a ﬁxed-bed column consisting of a Pyrex glass tube where a stainless-steel sieve was attached to the bottom followed by a layer of glass beads to provide a uniform ﬂow of the solution through the column. A known quantity of RF resin (10 g) was packed above the glass beads in the column consisting of 1.8 cm inner diameter to yield the desired bed height (6 cm). Feed solutions of 10 mg Sr/L with and without co-ions at concentrations that are found to occur in seawater (see Section 2.4.5) were pumped upward through the column at a desired ﬁltration velocity (10.6 mL/min, 2.5 m/h) which was controlled by a peristaltic pump. The experiment was deliberately conducted with a shorter bed height to obtain a faster breakthrough of metals. Since a shorter bed height was used, a smaller ﬁltration velocity was used instead of a normally used velocity of 10 m/h. The eﬄuents at the outlet of the column were collected at regular time intervals and the Sr concentrations were measured. The breakthrough curve shows the loading behaviour of Sr to be removed from the solution in the column and is usually expressed in terms of adsorbed Sr concentration (Cad), inlet Sr concentration (Co), outlet Sr concentration (C) or normalised concentration deﬁned as the ratio of outlet Sr concentration to inlet Sr concentration (C/Co) as a function of time. The maximum column adsorption capacity, qtotal (meq of Sr/g), for a given feed concentration and ﬁltration velocity is equal to the area under the plot of the adsorbed Sr concentration, Cad (Cad = CoC) (meq/L) versus eﬄuent time (t, min) and was calculated manually using Microsoft Excel spreadsheet according to Eq. (7).
2.4.3. K, Ca, and Mg adsorption The adsorption of K, Ca, and Mg on RF was investigated in experiments similar to that described previously for Sr adsorption with initial cations concentration of 10 mg/L at RF doses of 0.1–10 g/L. The adsorption data for these metals and Sr were ﬁtted to the Langmuir model (Eq. (6)).
qmax KL Ce 1 + KL Ce
where, Qe = amount of metal adsorption (meq/g) at the equilibrium metal concentration Ce (meq/L), qmax = maximum amount of the metal adsorption (meq/g), KL = Langmuir adsorption constant (L/ meq). 2.4.4. Eﬀect of pH on Sr adsorption The eﬀect of pH on Sr adsorption was investigated by adding 0.05 g RF resin to 100 mL solution containing 10 mg Sr/L and the suspension was shaken in a ﬂat shaker with a shaking speed of 120 rpm at room temperature (24 ± 1 °C) for 24 h. The solutions' pH values were initially set at a range of 2.5–10.0 using 0.1 M HCl and 0.1 M NaOH. They were adjusted back to their initial values after a shaking period lasting 4 h. The ﬁnal pHs at the end of the shaking period were measured. A HQ40d portable pH Meter was used for all pH measurements.
t = total
The breakthrough curves for the co-ions Ca, Mg and K were also determined by measuring their concentrations in the eﬄuent. The amounts of these metals adsorbed on RF were determined using Eq. (7). Equilibrium Sr uptake qeq (meq/g) or maximum Sr capacity of the column is qtotal divided by the mass of the adsorbent. The column adsorption data were ﬁtted to the Thomas model (Eq. (8)) which has been described elsewhere .
2.4.5. Eﬀect of co-ions in seawater medium on Sr adsorption Three adsorption experiments were conducted to determine the eﬀect of co-ions on Sr adsorption. The ﬁrst experiment was conducted in synthetic seawater containing Na (20 g/L), Ca (1 g/L), Mg (2 g/L), K (0.85 g/L) and Sr (10 mg/L) with RF doses of 0.1–10 g/L. The second experiment was conducted by keeping the Sr concentration and RF dose ﬁxed at 10 mg/L and 1 g/L, respectively, but Na (20 g/L), Ca (1 g/L), Mg (2 g/L) or K (0.85 g/L) was added individually to separate Sr solutions. To determine the co-ions having the greatest inﬂuence on Sr adsorption, the third experiment was undertaken at three concentrations of Ca, Mg and K (10, 20, 40 mg/L) in the presence of a ﬁxed concentration of Sr (10 mg/L) at a RF resin dose of 1 g/L. This experiment is expected to provide information on the eﬀect of diﬀerent ratios of the concentrations of Sr to co-ions on Sr adsorption. The amount of Sr adsorption was calculated using Eq. (5).
ln (Co C − 1) = kThq o M Q − kThCo t
where, kTh is the Thomas rate constant (L/min·meq), qo is the maximum solid-phase concentration of the solute (meq/g), mc is the mass of adsorbent in the column (g), and Q is the volumetric ﬂow rate (L/min). kTh and qo were calculated from the model ﬁt to the data. The accuracy of the model ﬁt to the experimental data was determined by applying error analysis methods such as the sum of the squared error (SSE) and root mean squared error (RMSE) described in the following equations . 2
⎛ SSE = Σin= 1 yc − y ⎟⎞ ⎜ e⎠ ⎝
2.4.6. Selectivity of Sr adsorption on RF resin Another experiment was conducted to investigate the selectivity of Sr adsorption on RF resin when the same concentration of Sr, Ca, Mg and K (10 mg/L) was used at a RF resin dose of 1 g/L. The amount of each metal adsorbed was calculated using Eq. (5). The removal eﬃciency (%) of a metal ion by RF was determined by dividing the amount adsorbed by the amount initially present and multiplying by 100. The distribution coeﬃcient (Kd) (L/g) of a metal was calculated by dividing the amount of metal adsorbed (meq/g) by the equilibrium
RMSE = √Σin= 1 [(yc − ye )2] n
where, n is the number of experimental data points, yc is the predicted (calculated) data, ye is the experimental data, and y represents the ratio C/Co 2.6. Desorption Sr desorption experiments were conducted using 1 M and 2 M of 3
Desalination xxx (xxxx) xxx–xxx
T. Nur et al.
Removal efficiency (%)
80 60 RF Resin
4 6 Adsorbent dose (g/L)
Fig. 2. Sr adsorption isotherm for diﬀerent adsorbents (initial Sr concentration 10 mg/L, adsorbents doses 1–10 g/L, pH 7.5–8.5).
Fig. 1. FTIR spectra of RF resin.
towards Sr could be due to the increased number of negatively charged phenolate groups generated in the NaOH system as shown by the zeta potential data (Section 3.2.3). Another study showed that conditioning RF with elevated concentrations of NaOH in the presence of constant Na+ concentration maintained by a high concentration of NaNO3, increased the adsorption of Cs. This was explained as being due to increased ionisation of phenolic OH groups .
NaCl and NaOH as desorbing agents. The RF resin containing the adsorbed Sr was washed with MQ water and used for the desorption experiments. As with the Sr adsorption experiment, 1 g of the RF resin containing adsorbed Sr was added to 100 mL of the desorbing solution and agitated for 4 h and then the supernatant was ﬁltered using 0.12 mm syringe ﬁlters. The concentration of Sr in the desorbed solution was measured in the ﬁltrate.
3.2.2. Comparison of diﬀerent adsorbents for Sr adsorption The adsorption capacities of four commonly used adsorbents were compared with RF in an experiment on adsorption of Sr from a solution with Sr concentration of 10 mg/L. The results showed that of the ﬁve adsorbents tested, RF had the highest adsorption capacity (Fig. 2). Approximately 96% removal of Sr was achieved with a resin dose of 1 g/L and the removal eﬃciency reached 99% and 100% with resin doses of 5 g/L and 10 g/L, respectively. Under the same adsorption conditions, only Amberlite and AMP could achieve about 80% removal eﬃciency at doses ≥5 g/L.
3. Results and discussion 3.1. Characterisation of the materials The X-ray diﬀraction analysis showed that the RF resin had no diﬀraction peaks, indicating that the resin was poorly crystalline (amorphous) as reported previously . The FTIR spectrum of the RF resin is shown in Fig. 1. The broad FTIR absorption band at 2800–3500 cm− 1 and the peak at 1640 cm− 1 correspond to the symmetrical and anti-symmetrical stretching vibrations of water molecules with hydrogen bonding and free water, respectively. The absorption peak occurring at 1200–1500 cm− 1 is due to OH bending of the phenolic group and the characteristic of the phenyl group. The band at 1000–1150 cm− 1 is due to CeO stretching and the peak at 600–800 cm− 1 is assigned to the presence of aromatic rings. The FTIR pattern with the above characteristic peaks agreed with the previous results of RF resin . The ion exchange capacity of RF determined by the method of Banerjee et al.  was 7.0 ± 0.3 meq/g and that by the method of Samantha et al.  was 6.7 ± 0.2 meq/g. These values are very close to the values of 6.0–6.9 meq/g reported by others [23,26] for the ion exchange capacity of RF.
3.2.3. Eﬀect of pH on Sr adsorption The adsorption capacity of RF resin in the pH range of 2.5 to 10 revealed that pH exerted a strong eﬀect on Sr adsorption capacity (Fig. 3a). The adsorption capacity remained constant from pH 2.5 to 4.5 and thereafter an abrupt increase was observed up to pH 7.5 and then remained constant up to pH 9.5. Others have also reported that Sr had a sharp increase in adsorption capacity around neutral to slightly alkaline pH on other adsorbents [35,36]. Fig. 3b shows the variation of the zeta potential of RF resin as a function of solution pH and the point of zero charge (PZC, pH at which the net surface charge is zero) of RF to be approximately 3.0. This value agrees with the PZC value of pH 3.2 reported by Sun et al.  for phenol-formaldehyde resin that is closely related to the RF. The negative zeta potential, as in the case of the adsorption capacity, also abruptly increased with pH from pH 5 to 8 in the presence of NaCl and KCl. This indicates that the increase in Sr adsorption was due to the increase in the surface negative charge which attracted the positively charged Sr by electrostatic forces (non-speciﬁc adsorption or outersphere complexation ). However, Fig. 3b also indicated that in the presence of Sr, the zeta potential became less negative above pH 5 compared to RF in the presence of a similar concentration of NaCl (10− 3 M). The zeta potential value between pH 5 and 7.5 for Sr showed negligible change (Fig. 3(b)), yet the pH eﬀect on Sr adsorption capacity at this pH range showed a signiﬁcant increase (Fig. 3a). This suggests that Sr was adsorbed on RF by speciﬁc adsorption or inner-sphere complexation  and not driven entirely by the coulombic charge
3.2. Batch adsorption experiments 3.2.1. Comparison of the adsorption capacities of diﬀerent RF resins The results of adsorption experiments with virgin RF resin and RF resins conditioned with three metal hydroxides (1 M NaOH, 1 M KOH, 1 M Ca(OH)2) showed that the NaOH conditioned RF resin had higher Sr removal eﬃciency than the other resins and virgin RF resin. The Sr removal eﬃciencies for the RF resins conditioned by these three metal hydroxides were 95%, 50%, and 45%, respectively compared to 40% for the virgin RF resin at the dose of 1 g/L and initial Sr concentration of 10 mg/L (Fig. S1). Therefore, the RF resin conditioned with NaOH was used in the remaining adsorption experiments. The higher adsorption capacity of the NaOH conditioned RF 4
Desalination xxx (xxxx) xxx–xxx
T. Nur et al.
Adsorption capacity (meq/g)
1.2 0.8 0.4
5 6 Final pH
Zeta potential (mV)
3.2.4. Batch adsorption modelling The adsorption of Sr on RF showed that the data ﬁtted successfully to the Langmuir model (R2 = 0.98) (Fig. 4). The maximum adsorption capacity of 2.28 meq/g obtained from the data ﬁt to the Langmuir model is one of the highest Sr adsorption capacity values reported for adsorbents in the literature (Table 1). The data ﬁt to the Langmuir model indicates that the adsorption sites on RF were homogeneous with monolayer adsorption coverage. The adsorption capacity of Sr was much higher than that of the other divalent cations, Ca and Mg and the monovalent cation K (Fig. 4). The adsorption of Ca and Mg also ﬁtted well to the Langmuir adsorption model (R2 of 0.97 and 0.90, respectively) but the adsorption maxima calculated from the model for Ca of 1.25 meq/g and for Mg of 1.15 meq/g were much lower than that for Sr. This is consistent with the zeta potential data where the surface negative potential on RF decreased in the order Sr > Ca > Mg > K (Fig. 3b). This order reﬂects the extent of inner-sphere complexation of the cations on the RF surface in addition to the charge diﬀerence of the cations (monovalent K vs the divalent ions) controlling the adsorption capacities of the cations.
SrCl2 CaCl2 MgCl2
Fig. 4. Langmuir isotherm model ﬁts to data on adsorption of Sr, Ca, Mg and K on RF resin (initial concentration of Sr, Ca, Mg and K 10 mg/L, adsorbent doses of 0.1–1.0 g/L, pH = 7.5–8.5).
Final pH 3
KCl NaCl DI water
-40 Fig. 3. Eﬀect of (a) pH on Sr adsorption by RF resin and (b) zeta potential trend as a function of pH for alkali and alkaline earth metals (10− 3 M) and DI water (RF resin dose 0.5 g/L).
balance of the RF surface as dictated by outer-sphere complexation. Inner-sphere complexation may have occurred at neutral surface sites of the RF producing positive surface charges. Such surface complexation mechanism which had less correlation of Sr++ adsorption to surface charge development dominated the bonding between Sr++ and the FeOOH surface . The positive charges formed on RF surface balanced part of the surface negative charge resulting in a reduction in negative zeta potential. The sharp increase in adsorption from pH 4.5 to 7.5 was not considered to be due to adsorption of Sr(OH)+ species or surface precipitation of Sr(OH)2 as the formation of these species or precipitation do not occur below pH 11 [35,36]. The high Sr adsorption at high pH was explained as being due to complexation of Sr with the adsorbent's surface OH groups or by the mediation of the high concentration of OH– ions at high pH . Samanta and Misra  explained the higher aﬃnity of Cs towards resorcinol formaldehyde compared to other alkali metals as a consequence of the speciﬁc interaction of Cs with the phenolic OH groups of the resin. They stated that this was due to the weak hydration of Cs compared to the strong hydration of the smaller alkali metals. This explanation can also apply to Sr which has the lowest hydrated ionic radius (nm) (Sr 0.180, Ca 0.200, Mg 0.310)  and the lowest hydration energy (kJ/mol) (Sr −1524, Ca − 1657, Mg −2003)  among the alkaline earth metals. The low adsorption capacity of Sr at low pH is due to fewer negative charges on the RF resin surface as shown by the zeta potential data (Fig. 3b). Also, competition between Sr and the high concentration of protons could be involved in reducing the Sr adsorption capacity. Because of the high adsorption capacity of Sr at pH 7.5–8.5, the rest of the experiments were conducted at this pH range.
Table 1 Comparison of Langmuir adsorption capacity for Sr on RF resin with that on other adsorbents.
Adsorption capacity (meq Sr/g)
Bacteriogenic iron oxides Dolomite Hydrous ferric oxide Phosphate-modiﬁed montmorillonite Magnetic Fe3O4 particles modiﬁed sawdust (MCS) Moss biosorbent AMP–PAN Composite magnetic nanoparticles FeOOH (BT9) FeOOH (BT1) Strontium-ion imprinted hybrid gel Titanate nanotubes Alginate microspheres Titanosilicates RF resin
pH 7.0; 293 K pH 5.5; 293 K pH 10.0; 293 K pH 5.0; 298 K
0.01 0.03 0.16 0.29
   
pH 6.7; 293 K
pH 6.0; 293 K pH 5.0; 293 K pH 10.3; 298 K
0.30 0.36 0.45
  
pH 11.2; 288 K pH 10.5; 293 K pH 11.0; 293 K
0.62 0.75 1.76
  
pH 8.0; pH 8.0; pH 7.1; pH 7.5;
2.09 2.51 3.90 2.28
   This study
293 K 298 K 293 K 298 K
Desalination xxx (xxxx) xxx–xxx
0.2 Sr only Sr + Na Sr + K
Sr + Mg Sr + Ca
80 Adsprotion capacity
10 0 Sr
Fig. 5. Eﬀect of diﬀerent concentrations of co-existing ions on Sr adsorption by RF resin at the dose of 1 g/L (Sr concentration 10 mg/L).
Concentration of co-existing ions (mg/L)
Removal efficiency (%)
Adsorption capacity (meq/g)
Sr adsorption capacity (meq/g)
T. Nur et al.
Metal ions Fig. 6. Adsorption capacity and removal eﬃciency of metals (adsorption by RF resin at a dose of 1 g/L in the presence of all metal ions, each at a concentration of 10 mg/L).
3.2.5. Co-ions' eﬀect on Sr adsorption Information on the adsorption behaviour of Sr in the presence of other ions that are present in seawater is useful for the practical application of the adsorption process in recovering Sr from seawater. To obtain this information, an experiment was conducted on Sr adsorption in the presence of the major cations present in seawater such as Na, Ca, Mg and K at concentrations ranging from 10 mg/L to 40 mg/L while that of Sr was ﬁxed at 10 mg/L. The results showed that the adsorption capacity of Sr was not aﬀected by the presence of Na and K even at concentrations four times that of Sr (Fig. 5). However, in the presence of divalent cations, the Sr adsorption reduced by 4, 7, and 10% for Mg concentrations of 10, 20, and 40 mg/L, respectively and 8, 11, and 14% for the corresponding concentrations of Ca. This shows that the divalent Ca and Mg are competing with Sr for adsorption. Between the two ions, Ca reduced Sr adsorption more than Mg did at the same concentration expressed as mg/L which was also found for other Sr adsorbents . With Ca having a higher atomic weight of 40 than Mg of 24, at the same concentration of the two ions expressed as mmol/L, Ca would be even more competitive than Mg for Sr adsorption. Zeta potential data (Fig. 3(b)) where Ca reduced the negative zeta potential more than Mg did (Fig. 3(b)), is consistent with the relative competition outcomes of the two ions on Sr adsorption. The amounts of Ca and Mg adsorption at the same concentration of Sr of 10 mg/L were 0.37 meq/g and 0.90 meq/g, respectively compared to the adsorption of 0.27 meq/g of Sr (Table S1). However, the initial concentration of Sr expressed as mmol/L was 0.23 meq/L which was much lower than the values of 0.50 meq/L and 0.83 meq/L of Ca and Mg. Therefore, if the adsorption of the metals are compared at the same solution concentration expressed as mmol/L, the diﬀerence in the adsorption amounts may not be much diﬀerent between the metals. The monovalent K had less eﬀect on Sr adsorption than the divalent Ca and Mg because of the charge diﬀerence between the ions and the inner-sphere complexation behaviour of the divalent cations (Fig. 3b). The amount of K adsorbed at the same 10 mg/L solution concentration of K was 0.09 meq/g which is much lower than the amount of Sr adsorbed (0.27 meq/g) conﬁrming that K has less competitive eﬀect on Sr adsorption because K was adsorbed mainly by outer-sphere complexation as shown by the zeta potential results (Table S1).
higher with respect to K than the divalent metals, Ca and Mg. However, in determining the relative amounts of the metals' adsorption in practice, the relative concentrations of the metals in solution should also be considered. The selectivity of Sr compared to K is due to the higher valency of Sr(divalent) than K (monovalent) which caused stronger adsorption of Sr. The higher selectivity of Sr in relation to the other divalent alkaline earth metals, Ca and Mg is probably due to Sr having the lowest hydrated ionic radius (nm) (Sr 0.180, Ca 0.200, Mg 0.310)  and the lowest hydration energy (kJ/mol) (Sr − 1524, Ca − 1657, Mg −2003)  among the alkaline earth metals. Lower hydrated ionic radius and hydration energy leads to more speciﬁc interaction with RF . Zeta potential data showed that the surface negative potential on RF decreased in the order Sr > Ca > Mg > K indicating the order of the strength of adsorption (Fig. 3). 3.2.7. Sr adsorption in seawater medium To investigate the Sr adsorption behaviour of the RF resin in real seawater conditions, an experiment was conducted on Sr adsorption in synthetic seawater containing Na, Mg, Ca, K, and Sr concentrations (g/ L) of 20, 2, 1, 0.85, and 0.01, respectively. The RF resin demonstrated excellent eﬃciency of nearly 95% Sr recovery at a dose of 1 g/L in deionised water containing 10 mg/L of Sr (Fig. 7a). But the eﬃciency declined to about 40% in synthetic seawater medium with the same dose of adsorbent. However, the removal eﬃciency of other metals at the same dose of 1 g/L were < 10% (Fig. S2a). This indicates that at the same concentration of metals in solution, Sr might be adsorbed selectively compared to other metals. At this RF dose, the amounts of Sr, Ca, Mg and K adsorption were 0.16 meq/g, 3.0 meq/g, 3.0 meq/g and 0.26 meq/g, respectively (Fig. S2b). The higher adsorption capacities of the co-ions compared to Sr is due to the presence of other metals in the synthetic seawater at much higher concentrations than Sr. Similar results were reported with an alginate microsphere adsorbent where the Sr adsorption capacity was drastically reduced in seawater medium . Fig. 7b shows the Sr adsorption capacity of RF resin when each of the other metals was present individually at the concentrations they are found to occur in seawater. As found previously, Ca and Mg ions competed most with Sr adsorption on RF resin and much of the ion exchange sites were not available for the adsorption of Sr found in much lower concentrations. To avoid this competition, Ca and Mg can be removed prior to the adsorption process by removing them from seawater as CaCO3 and Mg(OH)2 precipitates, respectively .
3.2.6. Selectivity of Sr adsorption on RF resin The results of the selectivity experiment showed that the removal eﬃciency of Sr was higher than that of the other metals from solution containing all the four metals together (Fig. 6). The removal eﬃciency of Sr was about 80%, while those of Ca, Mg and K were 67%, 42% and 1%, respectively. The high removal eﬃciency of Sr resulted in a high Kd value of 0.079 (L/g) for Sr compared to 0.070, 0.054, and 0.001 for Ca, Mg, and K, respectively and selectivity coeﬃcients (Ks) for Sr with respect to Ca, Mg and K of 1.13, 1.46 and 79.0, respectively (Table S2). The Ks values of greater than one indicates that Sr is more selectively adsorbed on RF than the other metal. The selectivity is very much
3.2.8. Desorption Desorption of Sr from RF resin was studied to obtain information on the percentage of adsorbed Sr that can be recovered from the desorbed solution. Also, it was necessary to evaluate whether the adsorbent can be reused without any loss of Sr adsorption capacity. Sr desorption 6
Desalination xxx (xxxx) xxx–xxx
T. Nur et al.
Removal efficiency (%)
reaching a saturation of the column with Sr after 920 bed volumes (Fig. 8a). On the other hand, in the second experiment the breakthrough commenced from the start of the experiment and column saturation occurred much earlier (Fig. 8b). The breakthrough curve was steeper than in the ﬁrst experiment. This clearly shows that the co-ions at much higher concentrations than Sr as found in seawater competed with Sr adsorption on RF, thus conﬁrming the batch experimental results. It is interesting to note that in between 200 and 400 bed volumes, C/Co is almost constant. It might indicate preferential exchange of Ca and Mg on RF over Sr in this region. In the third experiment with no Ca and Mg in the inﬂuent solution, the breakthrough of Sr occurred after 200 bed volumes and the column became saturated later than in the second experiment (Fig. 8c). The adsorption capacities calculated from the breakthrough curves were 0.50, 0.14, and 0.25 meq/g in the ﬁrst, second and third experiments, respectively. The data ﬁtted very satisfactorily to Thomas model when only Sr was present in the inﬂuent solution (Fig. 8a). The model ﬁts to the data for Sr adsorption in the presence of other metals in the inﬂuent solution were not satisfactory (Fig. 8b, c), especially when Ca and Mg were present (Fig. 8b). This may be because of competition of Ca and Mg with Sr for adsorption on RF, which the Thomas model does not take into account. The error analysis of the model ﬁts to the data showed that both the SSE and RMSE were high when other metals were present with Sr, especially Ca and Mg (Table 2). The relationship between model predicted C/Co and experimental C/Co values was very good when only Sr was present (R2 = 0.93 and slope of the regression line matched the 1:1 line with slope 1) but not satisfactory when other metals were present (R2 = 0,64 and 0.76) (Table 2, Fig. S5). The adsorption capacities (meq/g) calculated from the model for the corresponding experiments were 0.46, 0.17 and 0.20 (Table 2), respectively. These values are approximately the same as those calculated manually from the breakthrough curves. The adsorption capacity of 0.46 meq/g with the feed solution of only Sr concentration of 10 mg/L is quite low compared to the Langmuir maximum capacity of 2.28 meq/g determined in the batch experiment. The main reason for this diﬀerence is that the ﬂow process used in the column experiment is never at equilibrium unlike in the batch experiments. A similar breakthrough capacity of 0.68 meq/g was reported for zeolite LTA-monoliths when Sr at the same concentration was passed through the monoliths . The breakthrough curves for the co-ions in the second experiment showed that these ions were also adsorbed simultaneously on RF in the column (Fig. S4). The C/Co values were lower for Sr compared to other metals at all bed volumes indicating that the ratio of metal adsorbed to metal concentration in solution was highest for Sr as found in the batch selectivity experiment (Section 3.2.6). However, the amount of Sr adsorbed on RF calculated from the breakthrough curve (0.14 meq/g) was lower than that of the co-ions (Mg 30 meq/g and Ca 5.4 meq/g) because of the much higher concentrations of these co-ions than Sr in the synthetic seawater. Despite K had much higher concentration than Sr in synthetic seawater medium, amount of K adsorbed (0.13 meq/g) was lower than Sr. This indicates that Sr has higher selectivity for adsorption than K as found in the batch selectivity experiment (Section 3.2.6).
80 60 40 Sr 10 mg/L
Sr 10 mg/L, Na 20 g/L, Ca 1 g/L, Mg 2 g/L, K 0.85 g/L
Sr adsorption capacity (meq/g)
4 6 Adsorbent dose (g/L)
Na(20 g/L) K (0.85 g/L) Mg(2 g/L)
Concentration of co-existing ions Fig. 7. (a) Removal eﬃciency of Sr by RF resin in D.I. water and seawater medium with diﬀerent doses of adsorbent and (b) eﬀect of co-existing seawater cations on Sr adsorption by RF resin (Sr 10 mg/L and adsorbent dose 1 g/L).
eﬃciency was tested with 1 M and 2 M NaCl and NaOH on a RF sample with adsorbed Sr. The Sr desorption eﬃciency was found to be higher with 2 M NaCl (100%) than with 1 M NaCl (90%) when 0.1 g RF with adsorbed Sr was shaken with 100 mL of NaCl for 3 h. In contrast, even a higher concentration of NaOH (2 M) could desorb only 30% of adsorbed Sr (Fig. S3). The ineﬃciency of the NaOH to desorb Sr is because of the high Sr adsorption in alkaline condition (Fig. 3). The weakly acidic phenolic –OH groups of the resin responsible for ion exchange were expected to fully realise their ion-exchange properties only if the –OH groups were ionised to the highest extent which occurred in alkaline solutions . At a lower pH produced by NaCl (pH 6.5), the adsorption of Sr is weaker and Na at the high concentration of 1 M and 2 M exchanged with Sr and the latter is eﬀectively desorbed.
3.3. Column study 4. Conclusions The results from the three column experiments are presented in the form of breakthrough curves in Fig. 8. The ﬁrst experiment had only Sr in the inﬂuent solution at a concentration of 10 mg/L. The second experiment had all the major metals at the concentrations present in seawater in the inﬂuent solution along with 10 mg/L of Sr. The third experiment was designed with the same inﬂuent concentrations as in experiment 2, but without Ca and Mg present. This experiment is expected to give information on the removal of Sr, if Ca and Mg are removed from the seawater by precipitation as CaCO3 and Mg(OH)2 prior to the RF adsorption process . In the ﬁrst experiment, the breakthrough of Sr occurred after 417 bed volumes and increasing concentration of Sr was found in the eﬄuent with increasing bed volumes
An RF resin synthesised by poly-condensation of formaldehyde and resorcinol followed by conditioning it with high concentration of NaOH had higher Sr adsorption capacity than RF resins conditioned with KOH and Ca(OH)2. Sr adsorption on the NaOH conditioned RF increased with pH reaching a maximum value at pH 7.5–8.5. The Langmuir Sr adsorption capacity for this resin at pH 7.5–8.5 was 2.28 meq/g which is among the highest values reported in the literature for other adsorbents. The adsorption capacity for the diﬀerent metals followed the order, Sr > Ca > Mg > K. The negative zeta potential of RF in the presence of Na markedly increased with pH but the rate of increase was much lower in the presence of Sr. Sr was adsorbed by both the outer7
Desalination xxx (xxxx) xxx–xxx
T. Nur et al.
Fig. 8. Breakthrough curves and Thomas model ﬁts to data on column adsorption of Sr with diﬀerent inﬂuents (a) Sr 10 mg/L, (b) Sr 10 mg/L, Na 20 g/L, Ca 1 g/L, Mg 2 g/L, K 0.85 g/L (c) Sr 10 mg/L, Na 20 g/L, K 0.85 g/L, (ﬁltration velocity 2.5 m/h and bed height 6 cm).
Table 2 The values for Thomas model parameters and error analysis of the model's ﬁt to the experimental data. Inﬂuent metals and concentrations
(a) Sr = 10 mg/L (b) Sr = 10 mg/L, Na = 20 g/L, Ca = 1 g/L, Mg = 2 g/L, K = 0.85 g/L (c) Sr = 10 mg/L, Na = 20 g/L, K = 0.85 g/L
Coeﬃcient of determination between model values and experimental values (R2)
sphere complexation and inner-sphere complexation whereas Na and K adsorption was mainly by outer-sphere complexation. Sr adsorption capacity was reduced in synthetic seawater containing high concentrations of Na, K, Ca, and Mg in both batch and column experiments. The reduction was mainly due to Ca and Mg. However, the selectivity coeﬃcient of Sr in the presence of K, Ca, and Mg when all metals were present together, each at the same concentration, was greater than one (1.13, 1.46, and 79 with respect to Ca, Mg, and K, respectively) suggesting that Sr was selectively adsorbed on RF. 1 M NaCl was found to be an eﬃcient reagent for the recovery of Sr adsorbed on RF and regeneration of the used RF for reuse. The study indicated that RF conditioned with NaOH is an attractive adsorbent for removing Sr from seawater, provided Ca and Mg are removed prior to the adsorption process probably by precipitating them as carbonate and hydroxide, respectively.
This work was funded by Australian Research Council Discovery Research Grant (DP150101377). Appendix A. Supplementary data Supplementary data to this article can be found online at http://dx. doi.org/10.1016/j.desal.2017.08.003. References  P. Loganathan, G. Naidu, S. Vigneswaran, Mining valuable minerals from seawater: a critical review, Environ. Sci. Water Res. Technol. 3 (2017) 37–53.  E.E. Angino, G.K. Billings, N. Andersen, Observed variations in the strontium concentration of sea water, Chem. Geol. 1 (1966) 145–153.
Desalination xxx (xxxx) xxx–xxx
T. Nur et al.  J.A. Ober, Strontium, US Geological Survey Mineral Commodity Summaries, US Geological Survey, 2013, pp. 156–157.  B. Ma, S. Oh, W.S. Shin, S.J. Choi, Removal of Co2 +, Sr2 + and Cs+ from aqueous solution by phosphate-modiﬁed montmorillonite (PMM), Desalination 276 (2011) 336–346.  S. Singh, S. Eapen, V. Thorat, C.P. Kaushik, K. Raj, S.F. D'souza, Phytoremediation of 137cesium and 90strontium from solutions and low-level nuclear waste by Vetiveria zizanoides, Ecotoxicol. Environ. Saf. 69 (2008) 306–311.  A. Sachse, A. Merceille, Y. Barré, A. Grandjean, F. Fajula, A. Galarneau, Macroporous LTA-monoliths for in-ﬂow removal of radioactive strontium from aqueous eﬄuents: application to the case of Fukushima, Microporous Mesoporous Mater. 164 (2012) 251–258.  K. Shozugawa, B. Riebe, C. Walther, A. Brandl, G. Steinhauser, Fukushima-derived radionuclides in sediments of the Japanese paciﬁc-ocean coast and various Japanese water samples (seawater, tap water, and coolant water of Fukushima Daiichi reactor unit 5), J. Radioanal. Nucl. Chem. 307 (2016) 1787–1793.  M. Nagaoka, H. Yokoyama, H. Fujita, M. Nakano, H. Watanabe, S. Sumiya, Spatial distribution of radionuclides in seabed sediments oﬀ Ibaraki coast after the Fukushima Daiichi nuclear power plant accident, J. Radioanal. Nucl. Chem. 303 (2015) 1305–1308.  U.S. Department of Health and Human Services, Toxicological Proﬁle for Strontium, Public Health Service, Agency for Toxic Substances and Disease Registry, Washington, DC, USA, 2004.  V. Höllriegl, H.Z. München, Strontium in the environment and possible human health eﬀects, in: J.O. Nriagu (Ed.), Encyclopedia of Environmental Health, Elsevier, Burlington, 2011, pp. 268–275.  C. Xu, J. Wang, J. Chen, Solvent extraction of strontium and cesium: a review of recent progress, Solvent Extr. Ion Exc. 30 (2012) 623–650.  A.D. Ebner, J.A. Ritter, J.D. Navratil, Adsorption of cesium, strontium, and cobalt ions on magnetite and a magnetite-silica composite, Ind. Eng. Chem. Res. 40 (2001) 1615–1623.  S. Chegrouche, A. Mellah, M. Barkat, Removal of strontium from aqueous solutions by adsorption onto activated carbon: kinetic and thermodynamic studies, Desalination 235 (2009) 306–318.  D.V. Marinin, G.N. Brown, Studies of sorbent/ion-exchange materials for the removal of radioactive strontium from liquid radioactive waste and high hardness groundwaters, Waste Manag. 20 (2000) 545–553.  Z.V.P. Murthy, S. Parmar, Removal of strontium by electrocoagulation using stainless steel and aluminium electrodes, Desalination 282 (2011) 63–67.  D.R. Raut, P.K. Mohapatra, V.K. Manchanda, A highly eﬃcient supported liquid membrane system for selective strontium separation leading to radioactive waste remediation, J. Membr. Sci. 390 (2012) 76–83.  P. Loganathan, S. Vigneswaran, J. Kandasamy, N.S. Bolan, Removal and recovery of phosphate from water using sorption, Crit. Rev. Environ. Sci. Technol. 44 (2014) 847–907.  T.D. Small, L.A. Warren, F.G. Ferris, Inﬂuence of ionic strength on strontium sorption to bacteria, Fe (III) oxide, and composite bacteria Fe (III) oxide surfaces, Appl. Geochem. 16 (2001) 939–946.  A. Ghaemi, M. Torab-Mostaedi, M. Ghannadi-Maragheh, Characterizations of strontium (II) and barium (II) adsorption from aqueous solutions using dolomite powder, J. Hazard. Mater. 190 (2011) 916–921.  Q. Li, H. Liu, T. Liu, M. Guo, B. Qing, X. Ye, Z. Wu, Strontium and calcium ion adsorption by molecularly imprinted hybrid gel, Chem. Eng. J. 157 (2010) 401–407.  H.J. Hong, J. Ryu, I.S. Park, T. Ryu, K.S. Chung, B.G. Kim, Investigation of the strontium (Sr (II)) adsorption of an alginate microsphere as a low-cost adsorbent for removal and recovery from seawater, J. Environ. Manag. 165 (2016) 263–270.  O. Oleksiienko, I. Levchuk, M. Sitarz, S. Meleshevych, V. Strelko, M. Sillanpää, Removal of strontium (Sr2 +) from aqueous solutions with titanosilicates obtained by the sol–gel method, J. Colloid Interface Sci. 438 (2015) 159–168.  S. Samanta, M. Ramaswamy, B. Misra, Studies on cesium uptake by phenolic resins, Sep. Sci. Technol. 27 (1992) 255–267.  C. Dwivedi, A. Kumar, J.K. Ajish, K.K. Singh, M. Kumar, P.K. Wattal, P.N. Bajaj, Resorcinol-formaldehyde coated XAD resin beads for removal of cesium ions from
radioactive waste: synthesis, sorption and kinetic studies, RSC Adv. 2 (2012) 5557–5564. J. Kaczvinsky, J. Fritz, D. Walker, M. Ebra, Synthesis and development of porous chelating polymers for the decontamination of nuclear waste, J. Radioanal. Nucl. Chem. 91 (1985) 349–360. D. Banerjee, R.A. Rao, P.K. Wattal, Separation and recovery of Cs from high activity waste simulant using resorcinol formaldehyde polycondensate resin: batch and column studies, Sep. Sci. Technol. 48 (2013) 133–139. E.A. Behrens, P. Sylvester, A. Clearﬁeld, Assessment of a sodium nonatitanate and pharmacosiderite-type ion exchangers for strontium and cesium removal from DOE waste simulants, Environ. Sci. Technol. 32 (1998) 101–107. D. Banerjee, M.A. Rao, S.K. Samanta, Evaluation of Amberlite IRC-718 chelating ion exchange resin in loading-elutionregeneration cycles for separation and recovery of strontium from alkaline radioactive waste, Solvent Extr. Ion Exch. 26 (2008) 687–698. Y. Park, Y. Lee, W.S. Shin, S. Choi, Removal of cobalt, strontium and cesium from radioactive laundry wastewater by ammonium molybdophosphate–polyacrylonitrile (AMP–PAN), Chem. Eng. J. 162 (2010) 685–695. S.K. Samanta, B.M. Misra, Ion exchange selectivity of a resorcinol-formaldehyde polycondensate resin for cesium in relation to other alkali metal ions, Solvent Extr. Ion Exch. 13 (1995) 575–589. J. Pan, X. Zou, Y. Yan, X. Wang, W. Guan, J. Han, X. Wu, An ion-imprinted polymer based on palygorskite as a sacriﬁcial support for selective removal of strontium (II), Appl. Clay Sci. 50 (2010) 260–265. T. Nur, W.G. Shim, P. Loganathan, S. Vigneswaran, J. Kandasamy, Nitrate removal using Purolite A520E ion exchange resin: batch and ﬁxed-bed column adsorption modelling, Int. J. Environ. Sci. Technol. 12 (2015) 1311–1320. J.J. García-Sánchez, M. Solache-Ríos, V. Martínez-Miranda, R. Enciso-Perez, N.V. Arteaga-Larios, M.C. Ojeda-Escamilla, I. Rodríguez-Torres, Experimental study of the adsorption of ﬂuoride by modiﬁed magnetite using a continuous ﬂow system and numerical simulation, Process. Saf. Environ. Prot. 109 (2017) 130–139. S.A. Shady, Selectivity of cesium from ﬁssion radionuclides using resorcinol–formaldehyde and zirconyl-molybdopyrophosphate as ion-exchangers, J. Hazard. Mater. 167 (2009) 947–952. C.H. Liu, Y.J. Shih, Y.H. Huang, C.P. Huang, Kinetic and thermodynamic studies for adsorptive removal of Sr2 + using waste iron oxide, J. Taiwan Inst. Chem. Eng. 45 (2014) 914–920. Y.J. Tu, C.F. You, Y.R. Chen, C.P. Huang, Y.H. Huang, Application of recycled iron oxide for adsorptive removal of strontium, J. Taiwan Inst. Chem. Eng. 53 (2015) 92–97. L. Sun, M. Li, M. Lin, B. Peng, J. Guo, Dispersion properties of a water-soluble phenol-formaldehyde resin, J. Dispers. Sci. Technol. 30 (2009) 605–608. K.G. Varshney, V. Jain, N. Tayal, Ion exchange kinetics of alkaline earth metals on acrylamide zirconium (IV) phosphate cation exchanger, Indian J. Chem. 41A (2002) 2318–2320. P.W. Atkins, J.A. Beran, General Chemistry, 2nd ed, Scientiﬁc American Books, New York, 1992. S. Langley, A.G. Gault, A. Ibrahim, Y. Takahashi, R. Renaud, D. Fortin, I.D. Clark, F.G. Ferris, Sorption of strontium onto bacteriogenic iron oxides, Environ. Sci. Technol. 43 (2009) 1008–1014. Z. Cheng, Z. Gao, W. Ma, Q. Sun, B. Wang, X. Wang, Preparation of magnetic Fe3O4 particles modiﬁed sawdust as the adsorbent to remove strontium ions, Chem. Eng. J. 209 (2012) 451–457. J. Marešová, M. Pipíška, M. Rozložník, M. Horník, L. Remenárová, J. Augustín, Cobalt and strontium sorption by moss biosorbent: modeling of single and binary metal systems, Desalination 266 (2011) 134–141. Y.J. Tu, C.F. You, Z. Zhang, Y. Duan, J. Fu, D. Xu, Strontium removal in seawater by means of composite magnetic nanoparticles derived from industrial sludge, Water 8 (2016) 357. J. Ryu, S. Kim, H.J. Hong, J. Hong, M. Kim, T. Ryu, I.S. Park, K.S. Chung, J.S. Jang, B.G. Kim, Strontium ion (Sr2 +) separation from seawater by hydrothermally structured titanate nanotubes: removal vs. recovery, Chem. Eng. J. 304 (2016) 503–510.